Search

Collections

Journals

About

Contact us

My IOPscience

Structure and spin dynamics of multiferroic BiFeO3

This content has been downloaded from IOPscience. Please scroll down to see the full text. 2014 J. Phys.: Condens. Matter 26 433202 (http://iopscience.iop.org/0953-8984/26/43/433202) View the table of contents for this issue, or go to the journal homepage for more

Download details: IP Address: 155.97.178.73 This content was downloaded on 09/10/2014 at 21:00

Please note that terms and conditions apply.

Journal of Physics: Condensed Matter J. Phys.: Condens. Matter 26 (2014) 433202 (33pp)

doi:10.1088/0953-8984/26/43/433202

Topical Review

Structure and spin dynamics of multiferroic BiFeO3 Je-Geun Park1,2 , Manh Duc Le1,2 , Jaehong Jeong1,2 and Sanghyun Lee3 1 2 3

Center for Correlated Electron Systems, Institute for Basic Science (IBS), Seoul 151-747, Korea Department of Physics and Astronomy, Seoul National University, Seoul 151-747, Korea Institute of Materials Structure Science, J-PARC Center, KEK, Tsukuba 305-0801, Japan

E-mail: [email protected] and [email protected] Received 23 July 2014, revised 24 August 2014 Accepted for publication 28 August 2014 Published 9 October 2014 Abstract

Multiferroic materials have attracted much interest due to the unusual coexistence of ferroelectric and (anti-)ferromagnetic ground states in a single compound. They offer an exciting platform for new physics and potentially novel devices. BiFeO3 is one of the most celebrated multiferroic materials and has highly desirable properties. It is the only known room-temperature multiferroic with TC ≈ 1100 K and TN ≈ 650 K, and exhibits one of the largest spontaneous electric polarisations, P ≈ 80 μC cm−2 . At the same time, it has a magnetic cycloid structure with an extremely long period of 620 Å, which arises from competition between the usual symmetric exchange interaction and the antisymmetric Dzyaloshinskii–Moriya (DM) interaction. There is also an intriguing interplay between the DM interaction and single ion anisotropy K. In this review, we have attempted to paint a complete picture of bulk BiFeO3 by summarising the structural and dynamic properties of both the spin and lattice parts and their magneto-electric coupling. Keywords: multiferroic, crystal structure, magnetic structure, BiFeO3 , magnetoelectric coupling, spin dynamics (Some ﬁgures may appear in colour only in the online journal) These multiferroics were ﬁrst studied in Russia by those interested in explaining the weak ferromagnetic component in Cr2 O3 , α-Fe2 O3 , MnCO3 , and FeBO3 [2–5]. Dzyaloshinskii famously discovered a new type of exchange interaction for materials without inversion symmetry. Moriya adopted the phenomenological form of the interaction proposed by Dzyaloshinskii and derived, from the superexchange theory of Anderson, microscopic expressions for their strength [6, 7]. This anisotropic exchange interaction, now known as the Dzyaloshinskii–Moriya (DM) interaction, can be written as HDM = D · Si × Sj with D as the DM vector and Si as the spin vector at the i site. The DM interaction is antisymmetric upon exchange of two spins, unlike the Heisenberg exchange interaction. While, in retrospect, this was an important point in the development of the theory of magnetism, foreshadowing later discoveries, it failed to attract the attention of the wider community outside Russia due to the relatively few materials

1. Introduction

When a solid is cooled, it often assumes one or another ordered states, including ferromagnetism and ferroelectricity, amongst others [1]. Usually, these phase transitions are driven by only one of the four fundamental degrees of freedom of a solid: the electronic charge, spin or orbital angular momentum, or the structure of the atomic lattice. The ordering is always accompanied by, and sometimes deﬁned by, the breaking of some symmetry elements of the solid. For example, ferromagnetism, the parallel ordering of electronic spins, breaks time reversal symmetry whereas ferroelectricity, a net ordering of dipolar charges, is produced by breaking inversion symmetry, such as by shifting charges off their centre of inversion. However, compared with the large number of materials exhibiting only one such type of phase transitions, materials showing two types of transitions, such as both ferromagnetism and ferroelectricity, are few. 0953-8984/14/433202+33$33.00

1

© 2014 IOP Publishing Ltd

Printed in the UK

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

which have spiral magnetic structures that break inversion symmetry, or mixed valent materials such as LuFe2 O4 [26] or Ca3 CoMnO6 [27], where the ferroelectric polarisation comes from the magnetically induced polar charge ordering. Of the many multiferroic systems thus found, several families in particular have drawn intense interest: hexagonal RMnO3 , orthorhombic (perovskite) RMnO3 and RMn2 O5 [18], and BiFeO3 . While orthorhombic RMnO3 and RMn2 O5 are attractive because they are type-II multiferroics with strong magnetoelectric couplings, the ordering occurs at quite low temperatures ( 22.8 MV cm−1 in BiFeO3 thin ﬁlms, whereupon the AFD octahedral rotation is suppressed. This high theoretically calculated ﬁeld is expected to be decreased in real world measurements due to inhomogeneities in samples that should enhance the effect of the ﬁeld on the polarisation [156]. At ﬁelds below this transition, a ﬁrst order isostructural transition between two Cc phases is predicted, which is identiﬁed with the experimentally determined ﬂop of the cycloidal plane when the applied ﬁeld (E > Ec ≈ 12 kV cm−1 ) changes the polarisation direction in BiFeO3 single crystals mentioned above [128, 153]. In addition, the cycloidal structure itself can give rise to an additional electronic contribution to the polarisation under the spin-current model proposed by Katsura, Nagaosa, and Balatsky [22] (and thus also termed the KNB model), where P ∝ rij × (Si × Sj ). A similar contribution was attributed to the ﬂexomagnetoelectric effect through an analogy between the Lifshitz invariant describing the cycloid in BiFeO3 and that describing the director of liquid crystals by Zvezdin et al [82, 88]. The Lifshitz invariant was found to arise from the DM interaction. The KNB model and the ﬂexomagnetoelectric effect can be thought of as the microscopic and macroscopic views of the same physical phenomenon, which results from the microscopic coupling of the cycloid to the polarisation. This means that the energy of the cycloid is minimised when the cycloidal plane includes P. Thus, when the applied electric ﬁeld switches the polarisation direction, the cycloid plane also ﬂops as a result. This effect was subsequently used to image the change in magnetic domains by an applied magnetic ﬁeld in polarised neutron diffraction measurements [157]. In addition to affecting the polarisation and magnetic cycloid plane, the electric ﬁeld is also predicted to change the AFD rotation. The combination of these effects leads to a rich (calculated) phase diagram with up to four different phases as a function of ﬁeld direction [156].

This kind of magnetoelectric coupling through a spin-lattice coupling has been shown to be rather strong in hexagonal RMnO3 [30, 153, 158, 159]. Therefore, it is also natural to look for such a possibility in BiFeO3 , which requires an accurate measurement of atomic positions. Some of earliest measurements were reported by several groups, including Palewicz et al, who conducted powder neutron diffraction measurements to obtain structural information such as the lattice constant, rhombohedral angle, and cation shifts [160]. According to their results, there is a clear change in the slope of the c lattice constant and rhombohedral angle near TN . Park et al also carried out synchrotron x-ray diffraction from 373 K to 895 K (in 6 K steps) in addition to single crystal neutron diffraction studies and conﬁrmed a similar anomaly in the temperature dependence of c and determined that the rhombohedral angle has a minimum slightly above TN [85]. Smirnova et al employed an ultrasonic pulsed-echo technique and found that the longitudinal elastic constant CL shows an anomaly slightly above TN [161]. These results, taken together, constitute strong evidence of a spin-lattice coupling. However, it is fair to say that despite these studies, the details of how the electric polarization is coupled to the antiferromagnetic order remains to be determined. To gain insights into the microscopic details of the magnetoelectric coupling, Lee et al carried out extensive studies of the temperature dependence of the crystal structure using the high-resolution single crystal neutron diffractometer, D9 at ILL, with a neutron wavelength of 0.835 Å , which is much shorter than the usual wavelength in neutron diffraction experiments [54]. Equipped with a wide area detector, this enabled us to examine the atomic positions with extremely high accuracy. The results were then used to calculate the cation shift directly and, ultimately, the electric polarization induced by the magnetic ordering. We should also stress that our ﬁndings of a noticeable magnetoelastic coupling below TN , but with a very weak temperature dependence in the atomic positions, are at variance with the claim of a strong temperature dependence in the atomic position made for 0.9BiFeO3 –0.1BaTiO3 [162]. As discussed above, BiFeO3 has the R3c structure denoted a+− a+− a+− in the Glazer tilting system. The anti-phase octahedral tilting does not break inversion symmetry and so cannot induce a polarization itself, while the Bi and Fe cation shifts are directly related to electric polarization. Therefore, these cation shifts can be taken as the order parameter of a Landau phase transition. It is important to note that one needs to distinguish between the nonmagnetic Bi shift (sc) and magnetic Fe shift (tc), and thus their respective contributions to a total electric polarization, to determine the magnetically induced polarisation change that we observed in the highresolution neutron diffraction studies. s and t denote the relative coordinates of Bi or Fe ions along c in hexagonal notation and sc and tc denote the shift with respects to their ideal positions in the cubic perovskite structure. Since the ferroelectric transition of BiFeO3 is of ﬁrst order, the free energy includes terms up to 6th order in the order parameter without a magnetoelectric coupling term and can be written as: α2 2 α4 4 α6 6 FBi,Fe = PBi,Fe + PBi,Fe + PBi,Fe , (9) 2 4 6

Apart from the external magnetic and electric ﬁeld, there is another way to examine the magnetoelectric coupling, namely via the change in polarisation as BiFeO3 becomes magnetically ordered. The N´eel transition is expected to be accompanied by ionic displacements, which can contribute to the electric polarisation.

3.4.3. Evolution with temperature.

17

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

neutron diffraction studies. Therefore, one can conclude that the spin-lattice coupling through magnetic exchange-striction gives rise to a magnetoelectric coupling in BiFeO3 . Recent theoretical studies also conﬁrm such a magnetoelectric coupling via a spin-lattice coupling and their results seem to be in good agreement with our conclusions [163]. Finally, this spin-lattice coupling may also explain the reduction in the photostrictive effect observed in BiFeO3 when a magnetic ﬁeld is applied [164]. The visible light induced lattice change is thought to be due to a combination of the photovoltaic and piezoelectric effects, where the electric ﬁeld from an electron-hole pair excited by incident photons creates a strain in the crystal. An applied magnetic ﬁeld, however, may cause a counter-strain, opposing the photostriction via the spinlattice coupling. However, further theoretical work is required to establish this. 4. Magnons, phonons and electromagnons

Having extensively covered the crystal and magnetic structure of BiFeO3 , we now turn to the dynamic behaviour of atoms and electrons. The quantised excitations of the lattice or magnetic subsystem, namely phonons and magnons, are completely described by their dispersion relation ω(q), and a measurement of this can yield the interaction strengths (force constants and exchange constants) of the atoms and magnetic moments involved. These measurements may also be exquisitely sensitive to the symmetry of the atoms involved and thus may also contribute to knowledge of the atomic structure [115, 120, 146]. Finally, the magneto-electric coupling can also be studied by measuring the quantised excitations unique to multiferroics, namely electromagnons, which are hybrid excitations of the spins and lattice that have characteristics of both. The advantage of inelastic neutron scattering in measuring these disparate excitations is its ability to measure the full momentum dependence of the phonons or magnons, whereas the wavelength of light at the frequencies of these excitations is much larger than the distance between atoms, so that the momentum transfered by the photon to the sample is small enough to restrict optical spectroscopies to near the Brillouin zone centre. In addition, the large neutron-magnetic scattering cross-section compared to that of light is advantageous for measurements of the spin dynamics [165]. Thus, the exchange interactions were determined by neutron scattering as we describe below. However, the energy resolution of even state-of-the-art inelastic neutron spectrometers compares relatively poorly to THz spectroscopy at low energies, where the anisotropic Dzyaloshinskii–Moriya (DM) interaction and single-ion anisotropy (SIA) dominate. Thus, optical spectroscopic techniques, especially terahertz spectroscopy, has proven invaluable in determining these interactions in BiFeO3 . One aspect, unique to BiFeO3 , which facilitates this is the long period of the magnetic cycloid structure, which gives a small modulation wavevector q, and the mixing of modes at integer harmonics nq due to the DM interactions and SIA allowing such modes to probed by optical techniques [72, 74, 138, 166]. Furthermore, the hybrid electromagnons have only been seen

Figure 14. (a) and (b) Temperature dependence of the lattice

constants. The solid lines represent theoretical calculations using a Debye–Gr¨uneisen formula. (c) The anti-phase rotation angle ω of the oxygen octahedron. (d) The Bi (sc) and Fe (tc) shifts along the c-axis. The solid (dashed) lines are the theoretical curves for the ﬁrst-order ferroelectric order parameter based on the Ginzburg–Landau free energy analysis with (without) the magnetoelectric coupling term [54].

where PBi,Fe represents the electric polarization associated with Bi and Fe ions individually. The free energy can then be minimized for a given order parameter to obtain its theoretical temperature dependence, which can be compared with experimental values estimated by the measured Bi and Fe shifts. The accuracy of the measurements can be tested by calculating the electric polarization from the experimental results. If we assume that the ionic charges correspond to the nominal valences of Bi and Fe (+3), then our estimate of the total electric polarization is P = 73 μC cm−2 , which is comparable to the electric polarization measured on single crystals [43]. Of further interest, as shown in ﬁgure 14, the Bi shift follows the theoretical line of a ﬁrst order ferroelectric transition remarkably well whereas the Fe shifts clearly deviates from the theoretical line below the N´eel temperature. It was found that the Fe shift is reduced by about 0.007 Å at 300 K from the theoretical line without magnetoelectric coupling. Most interestingly, the reduced Fe shift amounts to a reduction in the polarization by as much as ΔP ∼ −0.4 μC cm−2 or ΔP /P ∼ −0.55%. We should stress that this polarization reduction is one order larger than what is expected from the inverse DM interaction. Moreover, the contribution due to the inverse DM interaction should be positive for the spin chirality determined from the circularly polarised x-ray scattering [134], and thus is opposite to what was found in our single crystal 18

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

with optical techniques in BiFeO3 because the polarised neutron measurements that would separate the spin and ionic components of these excitations are difﬁcult to conduct and require quite large single crystals. We now discuss magnetic excitations, followed by lattice dynamics, and end this section with electromagnons. 4.1. Magnon

Spin waves are the collective excitations of a magnetic ﬂuctuation in the spin structure, which can be quantized as a quasiparticle called a magnon with deﬁnite energy and momentum and possessing spin S = 1. The excitation is fully described by the magnon dispersion relation ω(q), a measurement of which is sufﬁcient to determine the underlying interactions governing the spin dynamics. These interactions include the nearest and next-nearest exchange, and Dzyaloshinskii–Moriya interactions and the single-ion anisotropy, and were ﬁrst included in a Hamiltonian to describe the high ﬁeld spin structure in a Monte Carlo calculation [86]. They were subsequently determined in detail by spectroscopic measurements [44, 60, 72, 74], as described in the next two subsections which cover, respectively, high and low energy spin dynamics.

Figure 15. The Fe–O–Fe and Fe–O–O–Fe paths for the superexchange interaction between the NN and NNN in the distorted FeO6 octahedra. Red and blue lines represent a short and long Fe–O bond, respectively.

with the boson operators bi and bi† obeying [bi , bj† ] = δij . In other words, the spin operator vector at position r can be expressed as √ br+ br† Trx = S/2 √ y Sr = Rx (QG · r) Tr , Tr = −i S/2 br − br† (12) Trz = S − br† br

4.1.1. High energy spin dynamics: super-exchange interaction.

The principal interactions, which determines the local G-type antiferromagnetic structure and high N´eel temperature (TN ≈ 650 K) in BiFeO3 , are the nearest- and next-nearest neighbour exchange interactions (denoted NN and NNN, respectively, in the subsequent discussion). Since the NN Fe–O–Fe bond has an angle close to 180◦ , this interaction is strongly antiferromagnetic, resulting in a structure in which nearest neighbouring spins align anti-parallel. The NNN interaction is also antiferromagnetic, and both interactions are shown in ﬁgure 15. Due to the requirement of sizeable single crystals, the magnon dispersion measurement, which could directly determine these interactions, was not completed until recently, when Jeong et al [44], for the ﬁrst time, reported the magnon spectrum across the full Brillouin zone using inelastic neutron scattering with a time-of-ﬂight spectrometer, and Matsuda et al [60] reported a similar study using a triple-axis spectrometer. The spin Hamiltonian including only the Heisenberg exchange interactions is given by: Hexch = JΔ Sr · Sr+Δ = J Sr · Sr+α + J Sr · Sr+β , r,Δ

r,α

where RX (θ ) is the rotation matrix about the x-axis, Tr is the spin operator vector deﬁned in a local frame, in which spins are directed to the positive z-direction, and QG is the magnetic propagation vector for the collinear G-type AFM state in BiFeO3 :

1 1 1 QG = [0 0 3]hex = . (13) 2 2 2 pc The dot product in the Hamiltonian is simply rewritten as Sr · Sr = TTr Rx (QG · Δ) Tr and the Hamiltonian can be rewritten as Hexch = JΔ cos (QG · Δ) S 2 − 2Sbr† br r,Δ

+

r,β

(10) where JΔ is the interaction parameter for neighbouring spins with the displacement vector Δ (See ﬁgure 15). Here, J = Jα and J = Jβ are for NN and NNN with the displacement vectors α and β, respectively. The magnon dispersion relation ω(q) and structure factor S(q, ω) can be calculated using the Holstein–Primakoff boson operators. Assuming a G-type antiferromagnetic (AFM) structure, the spin operators at two AFM sublattices can be written as S1z = S√− b1† b1 S1+ = √2Sb1 S1− = 2Sb1†

,

† S2z = −S √ + b†2 b2 + S2 = √2Sb2 S2− = 2Sb2

+

S JΔ [1 + cos (QG · Δ)] Kr,r+Δ 2 r,Δ

S JΔ [1 − cos (QG · Δ)] Pr,r+Δ 2 r,Δ

(14)

where Kr,r = br br† + br† br and Pr,r = br br + br† br† . Taking the Fourier transform 1 ik·r 1 −ik·r † br = √ e bk , br† = √ e bk , (15) N k N k the Hamiltonian can be rewritten as Ak † 2 Hexch = N S I0 +S bk b−k Bk

(11)

k

19

Bk Ak

bk , † b−k (16)

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

Figure 16. (a) The usual (gray) and conventional (black) hexagonal Brillouin zone. (b) Comparison with the pseudocubic Brillouin zone (blue). Red arrows denote the rhombohedral reciprocal vectors. (c) Full experimental magnon dispersion with J -only and J -J models indexed in hexagonal notation [44].

where the adapted high symmetry points M = ( 21 , 21 , 0)hex = ( 21 , 21¯ , 0)pc , K = ( 21 , 0, 0)hex = ( 13 , 23¯ , 13 )pc , and A = (0, 0, 23 )hex = ( 41 , 41 , 41 )pc suitable to the G-type Brillouin zone (shown in ﬁgure 16(a), are used rather than the usual hexagonal points M = ( 21 ,0,0)hex , K = ( 21 , 21 , 0)hex , and A = (0, 0, 21 )hex .5 The energy of the magnon at A is proportional to the total magnetic energy and thus is determined by the width of the magnon spectrum. It should also determine the N´eel temperature. From the data, ignoring the NNN interaction, a value

where 1 1 (Ik + Jk ) − I0 , Bk = (Jk − Ik ) , 2 2 Ik = JΔ cos (QG · Δ) cos (k · Δ) ,

Ak =

(17) (18)

Δ

Jk =

JΔ cos (k · Δ) .

(19)

Δ

Performing the Bogoliubov transformation bk γk cosh λk cosh λk = † † cosh λk cosh λk b−k γ−k

of J0 = 4.08 meV (with S =

(20)

k

k

(22)

where Ecl = NS 2 I0 is the classical ground-state energy, the second term gives an O(1/S) quantum correction to the energy, and 2Sωk is the magnon energy. Simple algebraic expressions can be obtained for the high symmetry points, shown in ﬁgure 16(a), and given by ωM = 4S 2 J0 2 − 2J0 J , (23) (24) ωK = 3S 3 J0 2 − J 2 , ωA = 6S(J − 2J ),

+ 1)) was determined,

which results in a Monte-Carlo estimate of TNMC = 620 K that is consistent with the measured N´eel temperature [86]. However, there are clear discrepancies between the measured and calculated dispersion in certain regions, including near the M point, which may be accounted for by including the NNN interaction, as shown in ﬁgure 16(c). In particular, the energy at the M point is the most crucial to determine J with a ﬁxed J0 . The best ﬁtting result is given by J = 4.38 and J = 0.15 meV [44, 60] with an antiferromagnetic NNN interaction. When the NN and NNN interactions are both antiferromagnetic, magnetic frustration can arise if the NNN is sufﬁciently strong. However, in this case, the G-type AFM state is stable since the condition J < J /4 is satisﬁed. Recent

with tanh 2λk = −Bk /Ak , the Hamiltonian is diagonalized as ωk + 2Sωk γk† γk , (21) Hexch = Ecl + S

ωk = A2k − Bk2 = (Jk − I0 ) (Ik − I0 ) ,

5 5 ( 2 2

5 Note that [44] uses the adapted G-type high symmetry points but without the prime notation.

(25) 20

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

Figure 17. The DM vectors (black arrows) for nearest neighbours on distorted octahedra and part of the spin cycloid (red arrows). The net effect of the DM interaction can be described by two effective DM vectors along two directions perpendicular to the cycloid direction: 1¯ 1 0 hex and [0 0 1]hex .

DFT calculation [102, 167] obtained a similar value for the NN interaction and conﬁrmed that the ground state is the G-type 1 AFM state with an NN to NNN interaction ratio ≈ 10 close to that determined by INS.

In BiFeO3 , the DM interaction between the nearest neighbours can be described by two effective DM terms, though the summation of the DM vectors is along the c-axis due to the 3-fold symmetry of the R3c crystal structure. As shown in ﬁgure 17, the DM interaction can be effectively rewritten as HDM = − DΔ · (Sr × Sr+Δ )

4.1.2. Low energy spin dynamics: DM interaction and singleion anisotropy. Although the simple Heisenberg Hamiltonian

r,Δ

discussed above describes the measured magnon dispersion quite well, the complex magnetic cycloid structure cannot be stabilised without the Dzyaloshinskii–Moriya (DM) interaction. Moreover, the single-ion anisotropy (SIA) is important, in that a large uniaxial anisotropy is expected to destroy the cycloid, whilst smaller values cause the cycloid to become anharmonic. Both these interactions come, in part, from perturbations induced by spin orbit coupling, and have a much smaller magnitude than the exchange interactions discussed above. Their effects are thus only apparent in the low energy magnon spectrum. Finally, the DM interaction in particular is also the microscopic origin of the Lifshitz invariant term in the free energy density [88] that is responsible for the non-linear magnetoelectric coupling between the cycloid and electric polarisation called by some authors the ﬂexomagnetoelectric interaction [82]. The DM interaction arises from the spin–orbit coupling that permits spin-ﬂip hopping between neighbouring ions, which leads, in a second order perturbation theory, to the antisymmetric exchange term Dij · Si × Sj [7]. The D coefﬁcient is only non-zero when the mid-point between spins Si and Sj is not at an inversion centre. This is satisﬁed in BiFeO3 below the ferroelectric transition due to the ferroelectric distortion that causes a displacement of the oxygen ligand in the Fe–O–Fe bond. The DM interaction tends to cause neighbouring spins to align perpendicular to each other and thus competes with the exchange interaction that favours their (anti-)parallel alignment, the result often being either a canting of the spins or, in the case of BiFeO3 , a long range cycloid.

=−

Du · (Sr × Sr+a vˆ ) −

r

Dc · Sr × Sr+ 2c cˆ

r

(26) with Du = Du uˆ working between the next nearest neighbors 6r·c along the v-axis and Dc = Dc (−1) c cˆ working alternately on ˆ vˆ , and cˆ are the unit different layers along the c-axis, where u, vectors along 1 1¯ 0 hex , [1 1 0]hex , and [0 0 1]hex , respectively. The ﬁrst term mainly produces the spin cycloid structure [55] propagating along the v-axis on the vc-plane, and the second term produces a spin density wave perpendicular to the cycloid plane [58]. The latter also induces weak ferromagnetism by canting the spins in the uv-plane when the spin cycloid is suppressed. The single ion anisotropy Hamiltonian is given by 2 Sr · cˆ , HSIA = −K (27) r

where the sign of K determines whether it is of an easyaxis (K > 0) or easy-plane (K < 0) form. Whilst the DM interaction is due mainly to the spin orbit coupling, the SIA comes mainly from an anisotropic deformation of the structure due to the spontaneous polarization in BiFeO3 . Recent DFT calculations [102] suggest that the competing antiferrodistortive (AFD) and ferroelectric (FE) distortions produce, respectively, easy-plane (AFD) and easy-axis (FE) anisotropies. The ﬁnal form of the SIA is then determined 21

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

where Φ is the canting angle out of the cycloid plane, which is responsible for the SDW with mr = 6r·ˆc/c. The corresponding spin operator vector is Sr = Rc (−1)mr Φ Ru (Q · r) Tr , (32)

by the relative amplitudes of these two distortions, which Weingart et al concluded to be of the easy-plane type with a magnitude of −1.3 μeV [102], in contrast to much of the literature, which assumes an easy-axis type anisotropy. A more recent DFT calculation found a magnetic easy axis with K = 3.5 μeV [163]. Moreover, the spin cycloid is no longer harmonic when the SIA is included as discussed in section 3. Whilst NMR and M¨ossbauer measurements [136, 168, 169] indicated that a large anharmonicity was present, this could not be measured by neutron diffraction [57, 131, 170, 171]. A precise measurement of the strength of the DM interaction and SIA would thus resolve this inconsistency. Finally, the measurements of Rovillain et al [155] and the theory of de Sousa et al [154] suggest that the SIA may be altered by an applied electric ﬁeld in a linear magnetoelectric effect, as discussed in section 3.4.2. There is thus a need for detailed measurements of the low energy spin dynamics, which has been fulﬁlled by studies using THz spectroscopy [74] and inelastic neutron scattering [59]. First, though, we discuss the linear spin wave theory needed to determine the effect of the DM interaction and SIA on the magnon dispersion. While the magnon dispersion for the full Hamiltonian (1) may be solved numerically in a linear spin wave theory by considering a large enough unit cell to encompass the full cycloid [72] using a spin rotation and Green function technique [172], this requires solving equations of motions for over 444 spins at each momentum transfer. On the other hand, if a harmonic cycloid is assumed (e.g. the SIA and DM term along c are ignored), the much simpler rotating frame operators in equation (12) may be used to ﬁnd an analytic solution. The corresponding spin operator vector can be written as Sr = Ru Qcyc · r Tr , where Ru (θ ) is the rotation matrix about the u-axis perpendicular to the cycloid plane and Qcyc = QG +Qm is the modulated magnetic propagation vector for the cycloid structure with (28) Qm = [δ δ 0]hex = δ δ¯ 0 pc

where Rc (φ) and Ru (θ ) are the rotation matrices about the cand u-axes, respectively. If, instead of considering a non-zero Dc , we consider the SIA in conjunction with the cycloid, then the spin operator vector becomes Sr = Ru (Q · r + φr ) Tr where φr is the modulation angle responsible for the anharmonicity of the cycloid caused by the SIA term. These approximations were termed models 1–5 by [59], with the corresponding magnon dispersion illustrated in ﬁgure 18(c). Model 1 (exchange interactions only) has a typical V-shape and the three possible modes which are detected by different components of S(q, ω) are degenerate. The induced spin cycloid in model 2 (exchange and Du nonzero) breaks this symmetry, so that the degenerate modes split into a phason mode and two spin-ﬂip modes corresponding to the in-plane and out-of-plane modes, respectively. This splitting of low energy magnon modes was theoretically expected [76]. Including the alternate DM interaction along the c-axis in model 3 mixes the modes at the wave vectors q and q ± Qm such that the dispersion lines are folded in a complex manner. However, the mixing amplitude becomes very small in the low-energy limit, so that there is little noticeable difference [59, 72, 74]. Finally, if this effect is ignored (Dc = 0) and the SIA is included instead (K = 0), as in models 4 (K > 0, easyaxis) and 5 (K < 0, easy-plane), the modes at q and q ± 2Qm are mixed, which changes the magnon dispersion signiﬁcantly [59, 72, 74]. The folded spectrum shows a large energy gap at the zone center. Moreover, there is a large difference between the forms of the SIA: easy-axis or easy-plane with respect to the c-axis [59]. As can be seen, the signiﬁcant changes caused by the DM and SIA terms are apparent only at the zone center at low energies. Because the mode splitting corresponds to the extremely small incommensurate modulation vector, it is very close to the original mode at the zone center. Although the full dispersion and exchange interactions could be determined by high-energy measurements, the effects of the DM interactions or the SIA are invisible within the limits of instrument resolution [44, 60]. Therefore, low-energy measurements at the zone center are critical to determine such small interactions. Several magnon modes at low frequency were measured using polarized Raman spectroscopy as shown in ﬁgure 19(a) [140, 141]. In principle, optical spectroscopy experiments only probe the modes close to the zone center because the velocity of light is high compared to the magnon velocity. However, magnon excitations in BiFeO3 at ﬁnite q can be measured due to magnon zone folding, which results from the DM interaction and SIA and thus the resultant small cycloid modulation wavevector. By choosing parallel and crossed polarizations, Cazayous et al successfully obtained two distinct species of spin excitations, called the cyclon (Φ , with spins oscillating within the cycloid plane) mode and the extra-cyclon (Ψ , spins oscillating out of the cycloid

where δ = 0.0045 in BiFeO3 . The ﬁrst term of equation (26) can be rewritten as u HDM =− Du sin Qcyc · λ S 2 − 2Sbr† br r

S + Du sin Qcyc · λ Kr,r+λ − Pr,r+λ 2 r

(29)

where λ = a vˆ is the displacement vector between adjacent spins along the cycloid direction. The ωk and S(ω, k) can be calculated following the same steps outlined in the previous section by replacing equation (18) with JΔ cos Qcyc · Δ cos (k · Δ) Ik = Δ

− Du sin Qcyc · λ cos (k · λ) .

(30)

A non-zero Dc introduces a canting of the cycloid with a classical ground state given by ⎞ ⎛ (−1)mr sin Φ sin Qcyc· r ⎠ , cos Φ sin Sr = S ⎝ (31) Qcyc· r cos Qcyc · r 22

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

Figure 18. (a) Theoretical spin wave spectra for a cycloid multiferroic without the anisotropy term. The solid and dashed lines are for

propagation along the direction perpendicular to the cycloid plane and along the polarization direction, respectively. The modes at nq are labeled by φn (cyclon) and ψn (extracyclon) for the in-plane and out-of-plane excitations, respectively. Reprinted with permission from [76]. Copyright 2008, American Physical Society. (b) The spin wave modes calculated with the full spin Hamiltonian equation (1) along [η η 0]pc from ( 21 , 21 , 21 )pc . The dashed lines show all possible excitations. Reprinted with permission from [73]. Copyright 2013, American Physical Society. (c) Calculated magnon dispersion along [h 0 0]hex near (1, 0, 1)hex for several models described in the text [59].

plane) mode [140]. As shown in the inset of ﬁgure 19(a), the Φ modes are equally spaced starting at zero energy, while the Ψ modes is not regularly spaced as expected by [76]. The cyclon and extra-cyclon modes correspond to the gapless phason and gapped spin-ﬂip modes mentioned above. The small gap of the out-of-plane modes can be explained by the energy cost for pinning of the cycloid plane. The mode splitting was conﬁrmed and its temperature dependence was studied by THz absorption measurements [138] with the additional mode splitting attributed to an additional DM term FDM = DPz (My Lx − Mx Ly ) corresponding the second effective DM term in equation (26). Combining the high and low energy measurement, the full set of parameters for the Hamiltonian (1) were determined using both INS and THz spectroscopy [59, 60, 72, 74, 166] as: J = 4.38, J = 0.15, Du = 0.11, Dc = 0.05, K = 0.003 meV. Thus the SIA is measured to be small but of the easy-axis form (K > 0), in contrast to the DFT calculation of [102], albeit the magnitude of the anisotropy constant is consistent. In addition, Weingart et al also assumed a DM vector parallel to the c-axis, which is inconsistent with the experimental ﬁndings. We note that the magnitudes of these terms are quite small, so that even extremely precise DFT calculations may not accurately determine them. Furthermore the SIA is, in the calculations, sensitive to the competition of the AFD and FE distortions, which results in a near cancellation of the SIA. Thus, it may be that the calculations slightly overestimate the

AFD and underestimates the FE distortions compared to the physical system. The magnetic ﬁeld [73, 166] and temperature [59] dependence of the magnon modes have also been reported. The modes, identiﬁed from IR measurements, soften as a function of the applied ﬁeld until the critical ﬁeld, where the cycloid is destroyed. Thereafter, a linear ﬁeld dependence of the magnon energies was observed, as shown in ﬁgure 20(a). Both observations are well-described by the full Hamiltonian (1) and in large part ﬁx the parameters noted above. In particular, whilst the second DM (Dc ) term has little effect on the inelastic neutron spectrum, it is very important in determining the ﬁeld dependence of the magnon modes above the critical ﬁeld and also in understanding the meta-magnetic phase above the spinﬂop transition [58, 73, 86]. As a function of temperature, inelastic neutron scattering measurements [59] showed systematic changes in the spectrum, which, when ﬁtted to the dispersion calculated from linear spin wave theory, allows the temperature dependence of the parameters of the Hamiltonian to be deduced. With increasing temperature, there is an apparent increase and then decrease in the energy of the minima in the scattering intensity, as shown by the right dotted line in ﬁgure 20(b). This corresponds to a change in the gap between the phason and spin ﬂip modes due to the single ion anisotropy. In addition, the initial maxima decreases slightly with increasing temperature (shown by the left dotted line in the ﬁgure), corresponding to a slight decrease of the DM interaction. This correlates with the 23

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

Figure 19. (a) Raman spectra of spin excitations. The Ψ and Φ cycloidal modes were selected using parallel (red) and crossed (blue) polarizations. Reprinted with permission from [140]. Copyright 2008, American Physical Society. (b) Temperature dependence of the magnetic resonance modes measured by the THz transmission. Inset: geometry of the measurement. Reprinted with permission from [138]. Copyright 2011, American Physical Society. (c) Low-energy magnon spectra at the magnetic zone center ( 21 , 21 , 21 )pc using cold neutron TAS. Reprinted with permission from [60]. Copyright 2012, American Physical Society. (d) Measured (left) and simulated (middle) low-energy magnon dispersions along [1 0 0]hex direction near the magnetic zone center (1, 0, 1)pc . Right: measured constant q-scan at (1, 0, 1)pc with the best ﬁt [59].

decrease of the cycloid period observed in neutron diffraction measurements [57]. The temperature dependence of the SIA may also be explained by deformations of the FeO6 octahedra. Finally, the scattered intensity falls with rising temperature in line with the measured magnetic moment. However, since the neutron scattering spectrum is quite insensitive to the effect of Dc , its temperature dependence could not be determined. As explained previously in section 3, and further in appendix B, the anharmonicity parameter m may be obtained from the parameters of the microscopic spin Hamiltonian (or equivalently the Landau–Ginzburg free energy density). Using the parameters deduced above from the neutron spectroscopies, a value of m ≈ 0.58–0.64 was found, from which an intensity 1 ratio of the third harmonic to the ﬁrst harmonic of 300 [59] can be deduced, in good agreement with the diffraction result [57], although this m value is larger than that estimated there.

to the underlying crystal structure. Phonon measurements, in combination with ab initio calculations, can thus allow the determination of the atomic motions that contribute to the ferroelectric order, and so provide insight into the nature of the ferroelectric transition. In the case of BiFeO3 , the lowest energy optic phonons are due to vibrations of Bi atoms [173]. Initial Raman spectroscopy measurements as a function of temperature [49, 117] showed that some of these modes decrease in energy as temperature increases, before abruptly disappearing above the ferroelectric transition. Ab initio calculations [174] showed that the motions of the lowest energy singly-degenerate transverse optic mode A1 (TO1 ) have a large overlap with the ferroelectric distortion, whilst the next highest A1 (TO2 ), which mainly involves FeO6 motions, corresponds to the AFD rotation. The ﬁrst reported Raman spectrum from single crystals [49, 117] and thin ﬁlms [175] yielded quite different zone centre phonon frequencies, in disagreement with each other. Latter Raman spectroscopy [176–179] and IR reﬂectivity or THz spectroscopy [118, 180] measurements supported that of [117], but introduced some confusion in the assignments of the symmetry of the modes. The trigonal point symmetry (C3v ) of the zone centre Γ -point of the R3c space group

4.2. Phonons

Just as the magnon spectrum is sensitive to the magnetic structure, so that the presence and anharmonicity of the cycloid lift the degeneracy of the magnon branches and alters their dispersion, the phonon spectrum is similarly sensitive 24

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

will be seen only in parallel polarisation (denoted z(xx)z and z(yy)z ) and not in cross-polarisation (z(xy)z and z(yx)z ). The E transverse optic (TO) modes will be seen in both polarisation channels. However, as noted by Beekman et al [179], a small misalignment of the laser polarisation with respect to the (111)pc face could yield A1 intensity in the cross-polarisation channel, and it is notably difﬁcult to polish BiFeO3 with a (111)pc face [175]. Additionally, the polishing itself could cause problems, for example, by creating multiple ferroelectric domains, each with a different orientation of the polarisation vector [117] or by inducing strain in the material, thus altering the phonons. Finally, when the phonon propagation vector deﬁned by the direction of the incident laser beam is not along a symmetry direction, oblique modes appear to disperse in frequency [178], which may also account for some of the variations in the reported phonon frequencies. The correct assignment of mode symmetries would allow a much better comparison between ab initio calculations and measurements, so that conclusions about the nature of the high temperature phase transitions could be more ﬁrmly drawn. To this end, Hlinka et al [178] and Beekman et al [179] offered two alternative methods to determine the mode symmetry. Hlinka et al [178] chose to take advantage of the dispersion of oblique modes by measuring the unpolarised micro Raman spectrum of over 70 randomly oriented single-crystalline grains, reasoning that the dispersion should be monotonic with the oblique angle φ, and that the E(TO) modes do not disperse. The spectra can thus be sorted in order of the measured phonon frequencies, with the lowest set of frequencies corresponding to the beam being parallel to [1 1 1]pc (φ = 0◦ ) and the highest frequency dispersed mode corresponding to the beam being perpendicular (φ = 90◦ ). The frequencies of the A1 (LO) modes can be determined from the φ = 0◦ spectrum, whilst the E(LO) and A1 (TO) modes from that with φ = 90◦ . Beekman et al [179], on the other hand, used the azimuthal polarisation dependence of the intensities of the modes to determine their symmetry, as reproduced in ﬁgure 21. This allowed them to reliably determine not just the mode symmetry, but also the Raman scattering tensors associated with each zone centre phonon mode, making a quantitative comparison with ab initio calculations possible. The experimental results, however, are at odds with the LSDA calculations of Hermet et al [174]. A better comparison between theory and experiments could be achieved when the full phonon dispersion is known, rather than just the zone centre frequencies that are accessible to optical spectroscopic techniques. Such a study was reported recently by Borissenko et al [121], who found good agreement between the measured inelastic x-ray scattering spectrum and calculated phonon dispersion curves (see ﬁgure 22). The LDA calculations in this case are very similar to that of [174], using the same functionals and pseudopotentials. Both sets of calculations do not, however, exactly reproduce the experimental crystal structure, so deviations between their predictions of the zone centre phonon frequencies and intensities indicate that these are particularly sensitive to slight differences in the structure. The same group also reported that using the recently proposed Wu–Cohen (WC) exchange-correlation

Figure 20. (a) Magnetic ﬁeld dependence of spin waves measured

by the THz absorption spectroscopy at low temperature. The vertical dashed line denotes the metamagnetic transition at Hc = 18.8 T. Reprinted with permission from [166]. Copyright 2013, American Physical Society. (b) Temperature dependence of low-energy magnon excitations with best ﬁt curves (left). Temperature dependence of interaction parameters and physical properties (right) [59].

means that there are three possible irreducible representations for the 27 possible phonon modes: the four non-degenerate A1 modes are Raman and IR active and polarised along the [1 1 1]pc direction (deﬁned as z for most measurements); the ﬁve non-degenerate A2 modes are silent; and the nine doubly degenerate E modes are Raman and IR active and polarised in the plane perpendicular to the electric polarisation (xy plane). In polarised Raman measurements, if the incident light is along the z direction, then the A1 longitudinal optic (LO) modes 25

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

Figure 21. Polar intensities determined from the Raman spectra as a function of azimuthal rotation. (a) and (b) A mode at 350 cm−1 . (c) and

(d) Ey mode at 140 cm−1 . (e) and (f ) Ex mode at 471 cm−1 . The solid red lines are ﬁts. Reprinted with permission from [179]. Copyright 2012, American Physical Society.

Figure 22. Experimental phonon dispersion curves (symbols) with ab initio calculation (line) along (a) [1 1 1]pc , (b) [1 1 0]pc , (c) [1 1 2]pc , and (d) [1 1¯ 0]pc directions. Open and full symbols correspond to transverse and longitudinal modes, respectively. Reprinted with permission from [121]. Copyright 2013, IOP Publishing. 26

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

functional in the generalised gradient approximation (GGA) or a hybrid functional (B1-WC), which mixes an exact exchange term together with the GGA–WC functional (with mixing parameter a0 = 0.16) [79], reproduces the experimental structure much more faithfully and also results in better agreement with the measured Raman frequencies. Thus, whilst the details of lattice dynamical properties of BiFeO3 require further theoretical work, the good agreement between the calculated and measured dispersion obtained by Borissenko et al [121] shows that broader conclusions may still be drawn from the data. This suggests that the low energy phonons, both those dominated by Bi vibrations and associated with the ferroelectric distortion and those at slightly higher energies associated with Fe motions and the AFD rotations [75, 174], may lay behind a displacive ﬁrst order ferroelectric transition. This view is supported by recent inelastic neutron scattering and GGA calculations of Zbiri et al [120], who obtained very good agreement between the measured and calculated generalised phonon density of states (gDOS). Their measured gDOS as a function of temperature is reproduced in ﬁgure 23 and shows clear, abrupt changes at the α → β and β → γ phase transitions, indicating that these are of ﬁrst order. In addition, it shows an incomplete softening of the low energy phonons around 10 meV (≈80 cm−1 ) as the sample is cooled in the β phase towards Tc . The data also shows the appearance of two strong peaks around 20 meV and 35 meV in the γ phase, which is linked to the disappearance of the oxygen modes at high energies and has been suggested to correspond to the breaking of Fe-O bonds, leading to a change of iron valence from (high spin) Fe3+ to (low spin) Fe2+ and thus to an insulator to metal transition. Figure 23. Temperature dependence of (a) diffraction patterns and (b) phonon gDOS spectra in the ferroelectirc α-phase (black), paraelectric β- (red) and γ -phases (blue). The transition temperatures, TN and TC , are highlighted in green. Reprinted with permission from [120]. Copyright 2012, American Institute of Physics.

4.3. Electromagnons and spin-lattice coupling

In addition to the phonons discussed above, optical spectroscopic techniques can also be used to measure zone centre magnons (called magnetic resonances in this context), which are excited by the oscillating magnetic ﬁeld of the incident photon. Whilst the intensities of these modes are sometimes much weaker than phonons, they can nevertheless often be detected. In multiferroics, furthermore, as a result of the magneto-electric coupling, a mixing of magnon and phonon excitations occurs, which results in hybrid magnonlike modes that can be excited by a photon’s electric ﬁeld (called electromagnons) and phonon-like modes that are excited by magnetic ﬁelds. In addition to mixing the modes, the magneto-electric coupling also shifts their frequencies with respect to the bare magnon or phonon frequencies. However, in BiFeO3 , these energy shifts are small [72, 76], so that, for example, magnetic resonances and electromagnons are coincident within experimental resolution. Electromagnons were ﬁrst reported by Singh et al [139], who found that the Raman spectrum of BiFeO3 showed a rich structure at low frequencies (70 cm−1 ) and that the temperature of the frequencies exhibited two anomalies at ≈140 K and ≈200 K. These transitions were subsequently determined to affect only the surface of the crystals as explained in section 3.3.3. Subsequent measurements and careful analysis of the polarisation dependence by Cazayous et al [140] showed that the modes

fell into two categories corresponding to the cyclon (denoted Φ ) and extra-cyclon (or spin-ﬂip, denoted Ψ ) magnetic excitations associated with ﬂuctuations of the moments in or out of the cycloidal plane, respectively. A theoretical treatment by de Sousa and Moore [76], using the Lifshitz invariant as the magnetoelectric coupling term, was found to satisfactorily account for the Raman observations. The plethora of modes (twelve were observed by Cazayous et al [140]) is due to the umklapp scattering of magnons outside the ﬁrst Brillouin zone, which is allowed due to the anharmonicity and periodicity of the cycloid. As noted by de Sousa and Moore [76] and Fishman et al [72], in a harmonic cycloid, where the single ion anisotropy K = 0, only one magnon (the Ψ1 mode) becomes electric dipole active. The other electromagnons arise only in the presence of anharmonicities of the cycloid (non-zero SIA), which allows the umklapp coupling between these magnons and a zero-wavevector phonon. In particular, de Sousa and Moore [76] determined that the Ψ3 and Φ2 modes should only become electric dipole active if the cycloid has a third harmonic. This is supported by THz spectroscopy measurements [138], 27

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

where the Ψ3 mode was only observable at low temperatures where the cycloid anharmonicity is more pronounced and a third harmonic is observed [58, 168], as shown in ﬁgure 19(b). In addition to making the cycloid anharmonic, the single ion anisotropy also splits the Ψn and Φn modes into two Ψ±n and Φ±n modes [72], with the splitting most pronounced for Ψ±1 . This splitting may be the source of initial confusion in the assignment of (electro)magnon modes from Raman scattering data, as the model of de Sousa and Moore does not explicitly include the SIA. Finally, an additional effective DM interaction along [1 1 1]pc is required to make the Ψ0 and Φ1 modes electric dipole active [74]. The models of both de Sousa and Moore [76] and Fishman et al [72, 74] relied on the Dzyaloshinskii–Moriya interaction to provide the necessary magneto-electric coupling to produce electromagnons. In the case of [76], this was given in the form of the Lifshitz invariant, the microscopic origin of which was shown by Zvezdin et al [88] to be from the DM interaction in conjunction with the AFD rotation and polar distortions of the FeO6 octahedron and Fe polar displacements. In the theory of Fishman et al, a coupling between the spin and electric polarisation was not explicitly included in the spin Hamiltonian, but the inverse DM mechanism was used to determine the electric dipole matrix elements (and hence oscillator strengths) of normally magnon modes. Thus, Fishman et al did not obtain any frequency shifts of electromagnons with respect to bare magnons, whereas de Sousa and Moore did. That the measured modes from Raman, IR, and THz spectroscopies agree well with the theory suggests that such shifts are small. The dynamical magnetoelectric coupling considered in these two theories thus bears similarities to the original model of electromagnons proposed by Katsura, Balatsky, and Nagaosa [181] and is distinct from the dynamic exchange-striction model [182], which is now thought to be responsible for the dominant electromagnons seen in the perovskite manganites such as TbMnO3 [183]. In that case it is a modulation of the symmetric Heisenberg exchange interaction by an incident electric ﬁeld which excites strong electromagnons. Finally, as mentioned in section 3.4.2, the magnetoelectric coupling proposed by de Sousa et al [154] in which an applied static electric ﬁeld enhances the single-ion anisotropy could also have strong effects on electromagnons by increasing the cycloid anharmonicities, potentially making more magnons electric dipole active, in addition to shifting the frequencies of the magnon modes, as was observed [155].

ever larger, this initial motivation has become gradually less important. Nonetheless, the lessons learnt from the physics of noncentrosymmetric materials are still relevant to several topics of current interest. Of the known multiferroic materials, BiFeO3 stands out for one reason alone: it is a room-temperature multiferroic system. Thanks to extensive research, summarised in part in this review, we now know an enormous amount of detail about the bulk properties of BiFeO3 . As such, there are only a few areas where further work appears necessary, amongst them the high temperature transitions between the paraelectric and ferroelectric phases, and the crystal structure within these phases, about which there is still some debate. The magnetic phase transition at 650 K has been well studied, as have the spin dynamics, such that we can now construct a full microscopic Hamiltonian that explains both the magnon dispersion and some structural aspects of the magnetic cycloid. Another major issue is magnetoelectric coupling. As we demonstrated in a high-resolution neutron diffraction study [54], there is clear evidence of a magnetoelectric coupling with a magnitude of a few hundred nC cm−2 , which seems to be consistent with theoretical calculations [163]. With this convincing result, it is probably a good time to think about how to maximize the effects in our favour. One area of further research may be doping experiments [184–186]. Although there have been some attempts in this direction, there is still much room for further exploration. Finally, it will also be instructive to observe the magneto-electric coupling in the spin dynamics, such as through a change in the magnon dispersion under an electric ﬁeld or the observation of an electromagnon. So far, all evidence of these excitations in BiFeO3 have come from optical measurements so it will be highly complementary to observe them by inelastic neutron scattering experiments and to examine their dispersion as well as their dynamical structure factor. Appendix A. Equivalence of the Landau–Ginzburg free energy and spin Hamiltonians

To compare the spin Hamiltonian (1) with the L–G free energy (2), let us consider the classical (magnetic) ground state and the corresponding energy. When the exchange interaction is dominant and the DM term is negligible, the ground state is a collinear order. Considering the collinear state, the ground state energy obtained from the spin Hamiltonian and the free energy are 2 H= JΔ Sr · Sr+Δ − K Sr · cˆ

5. Summary and outlook

r

Multiferroic materials are a class of systems with multiple coexisting ferroic phases. Of particular interest has been compounds that exhibit both ferroelectric and ferro- or antiferromagnetic phase transitions in a single compound. Initially, research was mainly driven by curiosity and the desire to ﬁnd new materials, which appeared to be rather rare among naturally occurring compounds when the subject resurfaced in late 1990s and its potential applications were recognised. However, as the list of multiferroic materials grows

Δ

= N S −3J + 6J − K cos2 θ , (A.1) 2 F = dV λl − Ku lc2 = V λ − Ku cos2 θ , (A.2) 2

where M0 is the magnitude of the sublattice magnetization vector Mi , l = (M1 − M2 )/2M0 is the antiferromagnetic unit vector, and θ is the angle between l and the c-axis. Clearly, λ < 0 or J > 0 for the AFM ground state and θ = 0 for an 28

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

easy-axis anisotropy Ku > 0 or K > 0. Here, we can ﬁnd the relations V λ = N S 2 −3J + 6J , (A.3) V Ku = N S 2 K.

where Φ is the canting angle and θ is the rotation angle on the cycloid plane. Whilst the ground state energy corresponding to other terms previously discussed is also changed in this state, the differences may be ignored for small Φ 1. The classical energies are now c HDM = − Dc sin φr+ 2c cˆ − φr sin2 θr (A.13)

(A.4)

The DM interaction favours a magnetic cycloid. If the small canting out of the cycloid plane and the SIA are ignored, the ground state is a harmonic cycloid that lies on the vc-plane. Considering the harmonic cycloid with Sr = S (0, sin θr , cos θr ) , θr = θ0 + Q · r,

=

r

FDM = −

(A.5)

= −

where Q = QG + Qm = (0.0045, 0.0045, 3)hex , the ground state energies are H= JΔ Sr · Sr+Δ − Du uˆ · (Sr × Sr+a vˆ ) r,Δ

dV 2βM0 Pz sin Φ cos Φ sin2 θ (A.15) dV βM0 Pz sin 2Φ sin2 θ,

V βM0 Pz = N S 2 Dc .

Δθ = NS −J 1 + 2 cos 2 Δθ +J 1 + 4 cos + cos Δθ + Du sin Δθ 2

J − 4J 2 ≈ NS 2 −3J + 6J + a (dv θ )2 + Du a (dv θ) , 4 (A.6) 2 2 F = dV λl + A (∇li )

f = fexch + fL + fan =A (∇li )2 − αP · [l (∇ · l) + l × (∇ × l)] − Ku lz2 , i=x,y,z

(8)

− α P · [l (∇ · l) + l × (∇ × l)]

where M0 is the magnitude of the magnetization vector Mi of the sublattices, P is the spontaneous polarization vector, and l = (M1 − M2 )/2M0 is the antiferromagnetic unit vector. The ﬁrst term is an exchange interaction term with the inhomogeneous exchange constant A (exchange stiffness), the second term is the Lifshitz invariant term with the inhomogeneous magnetoelectric (ﬂexomagnetoelectric) interaction constant α, and the last term is an uniaxial anisotropy term with the magnetic anisotropy constant Ku . Let l = (sin θ cos φ, sin θ sin φ, cos θ), so each term can be written as 2 fexch = A ∂i lj = A (∇θ )2 + sin2 θ (∇φ)2 , (B.1)

(A.7)

where Δθ = θr+a vˆ − θr = a(dv θ ) is the angle difference between spins along the cycloid direction [1 1 0]hex and P is the spontaneous polarization vector. Note that α > 0 or Du < 0 for the clockwise rotation and α < 0 or Du > 0 for the counterclockwise. Next, we can ﬁnd the relations J − 4J V A = N S 2a2 , (A.8) 4 V αPz = − N S 2 a Du .

(A.9)

i,j

The terms responsible for the canting out of the cycloid plane are 6 c HDM =− (−1) c r·ˆc Dc cˆ · Sr × Sr+ 2c cˆ , (A.10) FDM = −

fL = αPz lx ∂x lz + ly ∂y lz − lz ∂x lx − lz ∂y ly = − αPz cos φ (∂x θ) + sin φ ∂y θ − sin θ cos θ sin φ (∂x φ) − cos φ ∂y φ , (B.2)

r

dV 2βM0 P · (m × l),

(A.17)

To obtain the anharmonicity of the spin cycloid, we focus on the derivative (∇Li ) and the anisotropy terms, and ignore the small canting out of the cycloid plane. The corresponding LandauGinzburg free energy density can be then written as

= V λ + A (dv θ )2 − αPz (dv θ ) ,

(A.16)

Appendix B. Anharmonicity of the spin cycloid structure

2

i

(A.14)

so that we can ﬁnd the relation

r

r

Dc sin 2Φ sin2 θr ,

fan = − Ku lz2 = −Ku cos2 θ.

(A.11)

(B.3)

The Euler-Lagrange equations for f (θ, φ, ∂i θ, ∂i φ) can be derived as 2A ∇ 2 θ + 2αPz sin2 θ sin φ (∂x φ) − cos φ ∂y φ − sin 2θ A(∇φ)2 + Ku = 0, (B.4) 2 2A ∇ · sin θ (∇φ) − 2αPz sin2 θ sin φ (∂x θ) − cos φ ∂y θ = 0. (B.5)

where m = (M1 + M2 )/2M0 is the magnetization unit vector. Note that these vanish without a local ferromagnetic moment m. The ground state is the canted cycloid equation (31) or ⎛ ⎛ ⎞ ⎞ sin Φ sin θ sin Φ sin θ M1 M 2 = ⎝cos Φ sin θ ⎠ , = ⎝− cos Φ sin θ ⎠ , (A.12) M0 M0 cos θ − cos θ 29

J. Phys.: Condens. Matter 26 (2014) 433202

The solution is

Topical Review

∇φ = 0,

sin φ (∂x θ ) − cos φ ∂y θ = 0 ∂y θ φ = const = arctan ∂x θ 2 2A ∇ θ − Ku sin 2θ = 0

The shape of the anharmonic cycloid can be obtained in terms of the Jacobi elliptic function, ε Lz = cos ϕ = cn r, m (B.18) L m Lr ε = sin ϕ = sn r, m (B.19) L m

(B.6) (B.7) (B.8)

which gives a cycloid spin structure on the plane deﬁned by the z-axis and a direction in the xy-plane. The coordinate dependence of the angle θ generally exhibits nonlinear behavior due to equation (B.8). By rotating the coordinate system, so that θ (x, y) = θ (r), i.e. the cycloid lies in the rz-plane, it can be rewritten as d2 θ 2A 2 − Ku sin 2θ = 0. dr

for the easy-plane anisotropy (Ku < 0) and Lz π ε = cos ϕ − = sn r, m L 2 m Lr ε π = sin ϕ − = −cn r, m L 2 m

(B.9)

(B.21)

for the easy-axis anisotropy (Ku > 0). It can be rewritten with λ using the relation equation (B.15) as Lz 4K(m) Lr 4K(m) = cn r, m , = sn r, m (B.22) L λ L λ

This is the sine-Gordon equation for a nonlinear oscillator, which has two different solutions depending on the sign of Ku . θ, Ku < 0 ϕ= . (B.10) θ + π2 , Ku > 0

for the easy-plane anisotropy and Lz Lr 4K(m) 4K(m) = sn r, m , = −cn r, m L λ L λ

In both cases, the equation can be reduced to d2 ϕ ε + sin 2ϕ = 0, dr 2 2

(B.20)

(B.11)

where ε = |Ku |/A. We then obtain the solution by integrating this, following 2 dϕ + εsin2 ϕ = C, (B.12) dr dϕ ε 1 − msin2 ϕ, (B.13) =± dr m m r (ϕ) = ± F (ϕ, m) , (B.14) ε

(B.23)

for the easy-axis anisotropy. Acknowledgments

It has been our great pleasure to work with all of our collaborators over the past few years, who have enormously enriched our understanding of this unusual material. We would like to acknowledge a few people in particular for their help. First, we would like to thank S-W Cheong, who not only brought BiFeO3 to our attention (JGP), but also provided the high-quality single crystals that we used for the highresolution neutron scattering experiments. S Furukawa helped us in analyzing the spin waves and G Jeon carried out the Monte-Carlo simulation at the beginning of this project. Both have played an important role in helping us build a standard model of BiFeO3 , which was presented in this review. We also wish to thank Y Noda for his kind reading of the manuscript and comments, and J H Lee and R S Fishman for communicating their unpublished results to us. Finally, we acknowledge the authors of the papers from which we reproduced the ﬁgures used in this review and the publishers (APS, AIP, and IOP) for their generous permissions to reproduce such ﬁgures. Finally, whilst we have tried to be comprehensive, the large body of work on bulk BiFeO3 has inevitably meant that we have missed some publications. This work was supported by the Research Center Program of IBS (Institute for Basic Science) in Korea: Grant No. EM1203.

u| where C is the constant of integration, m ≡ Cε = |K and AC θ dθ √ is the incomplete elliptic integral of F (θ, m) = 0 2

1−msin θ

the ﬁrst kind with the parameter m. The period of the cycloid is m λ = r (2π ) − r (0) = 4 K (m) , (B.15) ε π/2 dθ where K (m) = F π2 , m = 0 √1−mcos is the complete 2θ elliptic integral of the ﬁrst kind. The anharmonicity parameter m can be obtained from this relation for given ε and λ. Note that m = 0 for Ku = 0 and approaches 1 for |Ku | A. The angle ϕ can be expressed by the Jacobi amplitude as the inverse of the incomplete elliptic integral, ε ε −1 ϕ (r) = F ± r, m = ±am r, m . (B.16) m m The two possible signs correspond to the winding direction of spins in the cycloid. Choosing a positive sign, ⎧ ⎪ |Ku | ⎪ r, m , Ku < 0 ⎨am Am θ (r) = . (B.17) ⎪ Ku π ⎪ r, m − , K > 0 ⎩am u 2 Am

References [1] Chaikin P M and Lubensky T C 2000 Principles of Condensed Matter Physics (Cambridge: Cambridge University Press) 30

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

[47] Kaczmarek W, Polomska M and Pajak Z 1974 Phys. Lett. A 47 227 [48] Kiselev S V, Ozerov R P and Zhdanov G S 1962 Dokl. Akad. Nauk SSSR 145 1255 Kiselev S V, Ozerov R P and Zhdanov G S 1962 Sov. Phys. Dokl. 7 742 [49] Haumont R, Kreisel J, Bouvier P and Hippert F 2006 Phys. Rev. 73 132101 [50] Selbach S M, Tybell T, Einarsrud M A and Grande T 2008 Adv. Mater. 20 3692 [51] Kornev I, Lisenkov S, Haumont R, Dkhil B and Bellaiche L 2007 Phys. Rev. Lett. 99 227602 [52] Arnold D, Knight K, Morrison F and Lightfoot P 2009 Phys. Rev. Lett. 102 027602 [53] Haumont R, Kornev I, Lisenkov S, Bellaiche L, Kreisel J and Dkhil B 2008 Phys. Rev. B 78 134108 [54] Lee S et al 2013 Phys. Rev. B 88 060103 [55] Sosnowska I and Zvezdin A 1995 J. Magn. Magn. Mater. 140–4 167 [56] Popov Y and Zvezdin A 1993 JETP Lett. 57 65 [57] Sosnowska I and Przeniosło R 2011 Phys. Rev. B 84 144404 [58] Ramazanoglu M, Laver M, Ratcliff W, Watson S M, Chen W C, Jackson A, Kothapalli K, Lee S, Cheong S W and Kiryukhin V 2011 Phys. Rev. Lett. 107 207206 [59] Jeong J, Le M D, Bourges P, Petit S, Furukawa S, Kim S A, Lee S, Cheong S W and Park J G 2014 Phys. Rev. Lett. 113 107202 [60] Matsuda M, Fishman R S, Hong T, Lee C H, Ushiyama T, Yanagisawa Y, Tomioka Y and Ito T 2012 Phys. Rev. Lett. 109 067205 [61] Neaton J B, Ederer C, Waghmare U V, Spaldin N A and Rabe K M 2005 Phys. Rev. B 71 14113 [62] Teague J R, Gerson R and James W 1970 Solid State. Commun. 8 1073 [63] Picozzi S and Ederer C 2009 J. Phys.: Condens. Matter 21 303201 [64] Ravindran P, Vidya R, Kjekshus A, Fjellvåg H and Eriksson O 2006 Phys. Rev. B 74 224412 [65] Di´eguez O, Gonz´alez-V´azquez O E, Wojdeł J C and ´Iniguez J 2011 Phys. Rev. B 83 094105 [66] Kornev I and Bellaiche L 2009 Phys. Rev. B 79 219902 [67] Albrecht D, Lisenkov S, Ren W, Rahmedov D, Kornev I A and Bellaiche L 2010 Phys. Rev. B 81 140401 [68] Rahmedov D, Wang D, ´Iniguez J and Bellaiche L 2012 Phys. Rev. Lett. 109 037207 [69] Zhdanov A G, Zvezdin A K, Pyatakov A P, Kosykh T B and Viehland D 2006 Phys. Solid State 48 88 [70] Tokunaga M, Azuma M and Shimakawa Y 2010 J. Phys. Soc. Japan 79 064713 [71] Gareeva Z V, Popkov A F, Soloviov S V and Zvezdin A K 2013 Phys. Rev. B 87 214413 [72] Fishman R S, Furukawa N, Haraldsen J T, Matsuda M and Miyahara S 2012 Phys. Rev. B 86 220402 [73] Fishman R S 2013 Phys. Rev. B 87 224419 [74] Fishman R, Haraldsen J, Furukawa N and Miyahara S 2013 Phys. Rev. B 87 134416 [75] Wang D, Weerasinghe J and Bellaiche L 2012 Phys. Rev. Lett. 109 067203 [76] de Sousa R and Moore J 2008 Phys. Rev. B 77 012406 [77] Zvezdin A K and Mukhin A A 2009 JETP Lett. 89 328 [78] Ederer C and Spaldin N 2005 Phys. Rev. B 71 060401 [79] Gofﬁnet M, Hermet P, Bilc D and Ghosez P 2009 Phys. Rev. B 79 014403 [80] Sparavigna A, Strigazzi A and Zvezdin A 1994 Phys. Rev. B 50 2953 [81] Tehranchi M M, Kubrakov N F and Zvezdin A K 1997 Ferroelectrics 204 181 [82] Zvezdin A K and Pyatakov A P 2009 Phys. Status Solidi 246 1956

[2] Dzyaloshinsky I 1959 Zh. Eksp. Teor. Fiz. 37 881 Dzyaloshinsky I 1960 Sov. Phys.—JETP 10 628 [3] Astrov D N 1960 Zh. Eksp. Teor. Fiz. 38 984 Astrov D N 1961 Sov. Phys.—JETP 11 708 [4] Smolenski˘i G A and Chupis I E 1982 Sov. Phys.—Usp. 25 475 [5] Venevtsev Y N and Gagulin V V 1994 Ferroelectrics 162 23 [6] Dzyaloshinsky I 1958 J. Phys. Chem. Solids 4 241 [7] Moriya T 1960 Phys. Rev. 120 91 [8] Schmid H 1994 Ferroelectrics 162 317 [9] Hill N A 2000 J. Phys. Chem. B 104 6694 [10] Spaldin N A and Fiebig M 2005 Science 309 391 [11] Eerenstein W, Mathur N D and Scott J F 2006 Nature 442 759 [12] Cheong S W and Mostovoy M 2007 Nat. Mater. 6 13 [13] Ramesh R and Spaldin N A 2007 Nat. Mater. 6 21 [14] Fiebig M 2005 J. Phys. D 38 R123 [15] Khomskii D 2006 J. Magn. Magn. Mater. 306 1 [16] Kimura T 2007 Ann. Rev. Mater. Res. 37 387 [17] Tokura Y and Seki S 2010 Adv. Mater. 22 1554 [18] Noda Y, Kimura H, Fukunaga M, Kobayashi S, Kagomiya I and Kohn K 2008 J. Phys.: Condens. Matter 20 434206 [19] Khomskii D I 2014 Transition Metal Compounds 1st edn (Cambridge: Cambridge University Press) [20] Sergienko I A and Dagotto E 2006 Phys. Rev. B 73 094434 [21] Arima T, Tokunaga A, Goto T, Kimura H, Noda Y and Tokura Y 2006 Phys. Rev. Lett. 96 097202 [22] Katsura H, Nagaosa N and Balatsky A V 2005 Phys. Rev. Lett. 95 057205 [23] Khomskii D 2009 Physics 2 20 [24] Kimura T, Goto T, Shintani H, Ishizaka K, Arima T and Tokura Y 2003 Nature 426 55 [25] Heyer O, Hollmann N, Klassen I, Jodlauk S, Bohat´y L, Becker P, Mydosh J A, Lorenz T and Khomskii D 2006 J. Phys.: Condens. Matter 18 L471 [26] Ikeda N et al 2005 Nature 436 1136 [27] Choi Y, Yi H, Lee S, Huang Q, Kiryukhin V and Cheong S W 2008 Phys. Rev. Lett. 100 047601 [28] Fiebig M, Degenhardt C and Pisarev R V 2002 J. Appl. Phys. 91 8867 [29] Lee S et al 2008 Nature 451 805 [30] Oh J, Le M, Jeong J, Lee J h, Woo H, Song W Y, Perring T, Buyers W, Cheong S W and Park J G 2013 Phys. Rev. Lett. 111 257202 [31] Ishiwara H 2012 Curr. Appl. Phys. 12 603 [32] Lebeugle D, Mougin A, Viret M, Colson D and Ranno L 2009 Phys. Rev. Lett. 103 257601 [33] Wang J et al 2003 Science 299 1719 [34] Ishiwata S, Taguchi Y, Murakawa H, Onose Y and Tokura Y 2008 Science 319 1643 [35] Kimura T, Lawes G and Ramirez A 2005 Phys. Rev. Lett. 94 137201 [36] Chun S H et al 2010 Phys. Rev. Lett. 104 037204 [37] Cheong S W 2014 private communication [38] Royen P and Swars K 1957 Angew. Chem. 69 779 [39] Lebeugle D, Colson D, Forget A, Viret M, Bonville P, Marucco J F and Fusil S 2007 Phys. Rev. B 76 024116 [40] Eerenstein W, Morrison F D, Dho J, Blamire M G, Scott J F and Mathur N D 2005 Science 307 1203 [41] Wang J et al 2005 Science 307 1203b [42] B´ea H, Bibes M, Petit S, Kreisel J and Barth´el´emy A 2007 Phil. Mag. Lett. 87 165 [43] Choi T, Lee S, Choi Y J, Kiryukhin V and Cheong S W 2009 Science 324 63 [44] Jeong J et al 2012 Phys. Rev. Lett. 108 077202 [45] Moreau J, Michel C, Gerson R and James W 1971 J. Phys. Chem. Solids 32 1315 [46] Roginskaya Y E, Tomashpol’skii Y Y, Venevtsev Y N, Petrov V and Zhdanov G 1966 Zh. Eksp. Teor. Fiz. 50 69 Roginskaya Y E, Tomashpol’skii Y Y, Venevtsev Y N, Petrov V and Zhdanov G 1966 Sov. Phys.—JETP 23 47 31

J. Phys.: Condens. Matter 26 (2014) 433202

[83] [84] [85] [86] [87] [88] [89] [90] [91] [92] [93] [94] [95] [96] [97] [98] [99] [100] [101] [102] [103] [104] [105] [106] [107] [108] [109] [110] [111] [112] [113] [114] [115] [116] [117]

[118]

Topical Review

[119] Delaire O, Stone M B, Ma J, Huq A, Gout D, Brown C, Wang K F and Ren Z F 2012 Phys. Rev. B 85 064405 [120] Zbiri M, Schober H, Choudhury N, Mittal R, Chaplot S L, Patwe S J, Achary S N and Tyagi A K 2012 Appl. Phys. Lett. 100 142901 [121] Borissenko E, Gofﬁnet M, Bosak A, Rovillain P, Cazayous M, Colson D, Ghosez P and Krisch M 2013 J. Phys.: Condens. Matter 25 102201 [122] Aroyo M I, Orobengoa D, de la Flor G, Tasci E S, Perez-Mato J M and Wondratschek H 2014 Acta Crystallogr. A 70 126 [123] Perez-Mato J M, Orobengoa D and Aroyo M I 2010 Acta Crystallogr. A 66 558 [124] Rodr´ıguez-Carvajal J 1993 Phys. B: Condens. Matter 192 55 [125] Orobengoa D, Capillas C, Aroyo M I and Perez-Mato J M 2009 J. Appl. Crystallogr. 42 820 [126] Fujii K, Kato H, Omoto K, Yashima M, Chen J and Xing X 2013 Phys. Chem. Chem. Phys. 15 6779 [127] Sosnowska I, Neumaier T P and Steichele E 1982 J. Phys. C 15 4835 [128] Lebeugle D, Colson D, Forget A, Viret M, Bataille A M and Gukasov A 2008 Phys. Rev. Lett. 100 227602 [129] Lee S, Ratcliff W, Cheong S W and Kiryukhin V 2008 Appl. Phys. Lett. 92 192906 [130] Herrero-Albillos J, Catalan G, Rodriguez-Velamazan J A, Viret M, Colson D and Scott J F 2010 J. Phys.: Condens. Matter 22 256001 [131] Ramazanoglu M, Ratcliff W, Choi Y J, Lee S, Cheong S W and Kiryukhin V 2011 Phys. Rev. B 83 174434 [132] Ramazanoglu M, Ratcliff W, Yi H T, Sirenko A A, Cheong S W and Kiryukhin V 2011 Phys. Rev. Lett. 107 067203 [133] Keffer F 1962 Phys. Rev. 126 896 [134] Johnson R D, Barone P, Bombardi A, Bean R J, Picozzi S, Radaelli P G, Oh Y S, Cheong S W and Chapon L C 2013 Phys. Rev. Lett. 110 217206 [135] Yamasaki Y, Sagayama H, Goto T, Matsuura M, Hirota K, Arima T and Tokura Y 2007 Phys. Rev. Lett. 98 147204 [136] Zalesskii A V, Zvezdin A K, Frolov A A and Bush A A 2000 JETP Lett. 71 465 [137] Pokatilov V S and Sigov A S 2010 J. Exp. Theor. Phys. 110 440 [138] Talbayev D, Trugman S A, Lee S, Yi H T, Cheong S W and Taylor A J 2011 Phys. Rev. B 83 094403 [139] Singh M K, Katiyar R S and Scott J F 2008 J. Phys.: Condens. Matter 20 252203 [140] Cazayous M, Gallais Y, Sacuto A, de Sousa R, Lebeugle D and Colson D 2008 Phys. Rev. Lett. 101 037601 [141] Rovillain P, Cazayous M, Gallais Y, Sacuto A, Lobo R, Lebeugle D and Colson D 2009 Phys. Rev. B 79 180411 [142] Redfern S A T, Wang C, Hong J W, Catalan G and Scott J F 2008 J. Phys.: Condens. Matter 20 452205 [143] Singh M K, Prellier W, Singh M P, Katiyar R S and Scott J F 2008 Phys. Rev. B 77 144403 [144] Palewicz A, Sosnowska I, Przeniosło R and Hewat A W 2010 Acta Phys. Pol. A 117 296 [145] Lu J, G¨unther A, Schrettle F, Mayr F, Krohns S, Lunkenheimer P, Pimenov A, Travkin V D, Mukhin A A and Loidl A 2010 Eur. Phys. J. B 75 451 [146] Jarrier R et al 2012 Phys. Rev. B 85 184104 [147] Mart´ı X, Ferrer P, Herrero-Albillos J, Narvaez J, Holy V, Barrett N, Alexe M and Catalan G 2011 Phys. Rev. Lett. 106 236101 [148] Jeon G 2010 private communication [149] Ruette B, Zvyagin S, Pyatakov A, Bush A, Li J, Belotelov V, Zvezdin A and Viehland D 2004 Phys. Rev. B 69 064114

Xu Z et al 2012 Phys. Rev. B 86 174419 Holstein T and Primakoff H 1940 Phys. Rev. 58 1098 Park J et al 2011 J. Phys. Soc. Japan 80 114714 Ohoyama K, Lee S, Yoshii S, Narumi Y, Morioka T, Nojiri H, Jeon G, Cheong S W and Park J G 2011 J. Phys. Soc. Japan 80 125001 Kadomtseva A M, Zvezdin A K, Popov Y F, Pyatakov A P and Vorob´ev G P 2004 JETP Lett. 79 571 Zvezdin A K and Pyatakov A P 2012 Europhys. Lett. 99 57003 Kubel F and Schmid H 1990 Acta Crystallogr. B 46 698 Goldschmidt V M 1926 Die Naturwissenschaften 14 477 Glazer A M 1972 Acta Crystallogr. B 28 3384 Glazer A M 1975 Acta Crystallogr. A 31 756 Lee S, Zhang J R, Torii S, Choi S, Cho D Y, Kamiyama T, Yu J, McEwen K A and Park J G 2013 J. Phys.: Condens. Matter 25 465601 Howard C J and Stokes H T 1998 Acta Crystallogr. B 54 782 Howard C J and Stokes H T 2002 Acta Crystallogr. B 58 565 Stokes H T, Kisi E H, Hatch D M and Howard C J 2002 Acta Crystallogr. B 58 934 Mitchell R H 2003 Perovskites: Modern and Ancient 1st edn (New York: Almaz) Islam M A, Rondinelli J M and Spanier J E 2013 J. Phys.: Condens. Matter 25 175902 Johnsson M and Lemmens P 2007 Handbook of Magnetism and Advanced Magnetic Materials (New York: Wiley) Zinenko V I and Pavlovski˘i M S 2009 Phys. Solid State 51 1404 Di´eguez O, Aguado-Puente P, Junquera J and ´Iniguez J 2013 Phys. Rev. B 87 024102 Weingart C, Spaldin N and Bousquet E 2012 Phys. Rev. B 86 094413 Zinenko V I and Pavlovskii M S 2008 JETP Lett. 87 288 Gonz´alez-V´azquez O and ´Iniguez J 2009 Phys. Rev. B 79 064102 Feng H 2010 J. Magn. Magn. Mater. 322 1765 Haumont R, Bouvier P, Pashkin A, Rabia K, Frank S, Dkhil B, Crichton W, Kuntscher C and Kreisel J 2009 Phys. Rev. B 79 184110 Guennou M, Bouvier P, Chen G S, Dkhil B, Haumont R, Garbarino G and Kreisel J 2011 Phys. Rev. B 84 174107 Zhang X L, Wu Y, Zhang Q, Dong J C, Wu X, Liu J, Wu Z Y and Chen D L 2013 Chin. Phys. C 37 128001 Hatt A J, Spaldin N A and Ederer C 2010 Phys. Rev. B 81 054109 Daumont C et al 2012 J. Phys.: Condens. Matter 24 162202 Sando D et al 2014 Phil. Trans. R. Soc. Lond. A 372 20120438 MacDougall G J, Christen H M, Siemons W, Biegalski M D, Zarestky J L, Liang S, Dagotto E and Nagler S E 2012 Phys. Rev. B 85 100406 Megaw H D and Darlington C N W 1975 Acta Crystallogr. A 31 161 Park J, Lee S, Lee S, Gozzo F, Cheong S W and Park J G 2008 unpublished Palai R, Katiyar R, Schmid H, Tissot P, Clark S, Robertson J, Redfern S, Catalan G and Scott J 2008 Phys. Rev. B 77 014110 Massa N E, del Campo L, de Souza Meneses D, Echegut P, Fabbris G F L, Azevedo G D M, Mart´ınez-Lope M J and Alonso J A 2010 J. Appl. Phys. 108 084114 Fukumura H, Matsui S, Harima H, Takahashi T, Itoh T, Kisoda K, Tamada M, Noguchi Y and Miyayama M 2007 J. Phys.: Condens. Matter 19 365224 ˇ Kamba S, Nuzhnyy D, Savinov M, Sebek J, Petzelt J, Prokleˇska J, Haumont R and Kreisel J 2007 Phys. Rev. B 75 024403 32

J. Phys.: Condens. Matter 26 (2014) 433202

Topical Review

[169] Palewicz A, Szumiata T, Przeniosło R, Sosnowska I and Margiolaki I 2006 Solid State Commun. 140 359 [170] Przeniosło R, Regulski M and Sosnowska I 2006 J. Phys. Soc. Japan 75 084718 [171] Przenioslo R, Palewicz A, Regulski M, Sosnowska I, Ibberson R M and Knight K S 2011 J. Phys.: Condens. Matter 23 279501 [172] Haraldsen J T and Fishman R S 2010 J. Phys.: Condens. Matter 22 509801 [173] Wang Y, Saal J E, Wu P, Wang J, Shang S, Liu Z K and Chen L Q 2011 Acta Mater. 59 4229 [174] Hermet P, Gofﬁnet M, Kreisel J and Ghosez P 2007 Phys. Rev. B 75 220102 [175] Singh M K, Jang H M, Ryu S and Jo M H 2006 Appl. Phys. Lett. 88 042907 [176] Kothari D, Raghavendra Reddy V, Sathe V, Gupta A, Banerjee A and Awasthi A 2008 J. Magn. Magn. Mater. 320 548 [177] Palai R, Schmid H, Scott J F and Katiyar R S 2010 Phys. Rev. B 81 064110 [178] Hlinka J, Pokorny J, Karimi S and Reaney I M 2011 Phys. Rev. B 83 020101 [179] Beekman C, Reijnders A A, Oh Y S, Cheong S W and Burch K S 2012 Phys. Rev. B 86 020403 [180] Lobo R, Moreira R, Lebeugle D and Colson D 2007 Phys. Rev. B 76 172105 [181] Katsura H, Balatsky A and Nagaosa N 2007 Phys. Rev. Lett. 98 027203 [182] Vald´es Aguilar R, Mostovoy M, Sushkov A, Zhang C, Choi Y, Cheong S W and Drew H 2009 Phys. Rev. Lett. 102 047203 [183] Shuvaev A M, Mukhin A A and Pimenov A 2011 J. Phys.: Condens. Matter 23 113201 [184] Do D, Bae Y, Kim J, Kim E, Kim G and Kim S 2011 J. Korean Phys. Soc. 59 2462 [185] Kim S, Han S, Kim H, Kim A, Kim J and Cheon C 2010 J. Korean Phys. Soc. 56 439 [186] Wu J, Wu W, Xiao D, Wang J, Yang Z, Peng Z, Chen Q and Zhu J 2012 Curr. Appl. Phys. 12 534

[150] Wardecki D, Przeniosło R, Sosnowska I, Skourski Y and Loewenhaupt M 2008 J. Phys. Soc. Japan 77 103709 [151] Popov Y F 2001 Low Temp. Phys. 27 478 [152] Tabares-Munoz C, Rivera J P, Bezinges A, Monnier A and Schmid H 1985 Japan. J. Appl. Phys. 24 1051 [153] Lee S, Choi T, Ratcliff W, Erwin R, Cheong S W and Kiryukhin V 2008 Phys. Rev. B 78 100101 [154] de Sousa R, Allen M and Cazayous M 2013 Phys. Rev. Lett. 110 267202 [155] Rovillain P, de Sousa R, Gallais Y, Sacuto A, M´easson M A, Colson D, Forget A, Bibes M, Barth´el´emy A and Cazayous M 2010 Nat. Mater. 9 975 [156] Lisenkov S, Kornev I and Bellaiche L 2009 Phys. Rev. B 79 012101 [157] Ratcliff W, Yamani Z, Anbusathaiah V, Gao T, Kienzle P, Cao H and Takeuchi I 2013 Phys. Rev. B 87 140405 [158] Fabr`eges X, Petit S, Mirebeau I, Pailh`es S, Pinsard L, Forget A, Fernandez-Diaz M and Porcher F 2009 Phys. Rev. Lett. 103 067204 [159] Park J et al 2010 Phys. Rev. B 82 054428 [160] Palewicz A, Przeniosło R, Sosnowska I and Hewat A W 2007 Acta Crystallogr. B 63 537 [161] Smirnova E P, Sotnikov A, Ktitorov S, Zaitseva N, Schmidt H and Weihnacht M 2011 Eur. Phys. J. B 83 39 [162] Singh A, Pandey V, Kotnala R and Pandey D 2008 Phys. Rev. Lett. 101 247602 [163] Lee J H and Fishman R S 2014 private communication [164] Kundys B, Viret M, Colson D and Kundys D O 2010 Nat. Mater. 9 803 [165] Jeong J, Lee S and Park J G 2012 J. Korean Magn. Soc. 22 103 [166] Nagel U, Fishman R S, Katuwal T, Engelkamp H, Talbayev D, Yi H T, Cheong S W and Room T 2013 Phys. Rev. Lett. 110 257201 [167] Kim H S and Yu J 2013 private communication [168] Zalesskii A V, Frolov A A, Zvezdin A K, Gippius A A, Morozova E N, Khozeevc D F, Bush A S and Pokatilov V S 2002 J. Exp. Theor. Phys. 95 101

33